General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 8.8 - 8.82 g/cm³ Show Material materials with Density of 8.8 - 8.82 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 182 GPa Show Material materials with Elastic modulus of 182 GPa |

100.0 °C | 180 GPa Show Material materials with Elastic modulus of 180 GPa | |

200.0 °C | 177 GPa Show Material materials with Elastic modulus of 177 GPa | |

300.0 °C | 170 GPa Show Material materials with Elastic modulus of 170 GPa | |

400.0 °C | 165 GPa Show Material materials with Elastic modulus of 165 GPa | |

500.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | |

Elongation | 20.0 °C | 30 - 35 % Show Material materials with Elongation of 30 - 35 % |

100.0 °C | 30 % Show Material materials with Elongation of 30 % | |

200.0 °C | 30 % Show Material materials with Elongation of 30 % | |

300.0 °C | 30 % Show Material materials with Elongation of 30 % | |

400.0 °C | 30 % Show Material materials with Elongation of 30 % | |

425.0 °C | 30 % Show Material materials with Elongation of 30 % | |

Unlock all property charts | ||

Elongation A100 | 20.0 °C | 20 - 30 % Show Material materials with Elongation A100 of 20 - 30 % |

Elongation A50 | 20.0 °C | 30 % Show Material materials with Elongation A50 of 30 % |

Hardness, Brinell | 20.0 °C | 140 - 150 [-] Show Material materials with Hardness, Brinell of 140 - 150 [-] |

Hardness, Vickers, 10 | 20.0 °C | 155 [-] Show Material materials with Hardness, Vickers, 10 of 155 [-] |

Shear strength | 20.0 °C | 340 MPa Show Material materials with Shear strength of 340 MPa |

Tensile strength | 20.0 °C | 400 - 730 MPa Show Material materials with Tensile strength of 400 - 730 MPa |

100.0 °C | 420 MPa Show Material materials with Tensile strength of 420 MPa | |

150.0 °C | 400 MPa Show Material materials with Tensile strength of 400 MPa | |

200.0 °C | 390 MPa Show Material materials with Tensile strength of 390 MPa | |

250.0 °C | 385 MPa Show Material materials with Tensile strength of 385 MPa | |

300.0 °C | 380 MPa Show Material materials with Tensile strength of 380 MPa | |

350.0 °C | 375 MPa Show Material materials with Tensile strength of 375 MPa | |

400.0 °C | 370 MPa Show Material materials with Tensile strength of 370 MPa | |

425.0 °C | 360 - 370 MPa Show Material materials with Tensile strength of 360 - 370 MPa | |

Unlock all property charts | ||

Tensile strength, transverse | 100.0 °C | 420 MPa Show Material materials with Tensile strength, transverse of 420 MPa |

150.0 °C | 400 MPa Show Material materials with Tensile strength, transverse of 400 MPa | |

200.0 °C | 390 MPa Show Material materials with Tensile strength, transverse of 390 MPa | |

250.0 °C | 385 MPa Show Material materials with Tensile strength, transverse of 385 MPa | |

300.0 °C | 380 MPa Show Material materials with Tensile strength, transverse of 380 MPa | |

350.0 °C | 375 MPa Show Material materials with Tensile strength, transverse of 375 MPa | |

400.0 °C | 370 MPa Show Material materials with Tensile strength, transverse of 370 MPa | |

425.0 °C | 370 MPa Show Material materials with Tensile strength, transverse of 370 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2 | 20.0 °C | 150 - 180 MPa Show Material materials with Yield strength Rp0.2 of 150 - 180 MPa |

100.0 °C | 150 MPa Show Material materials with Yield strength Rp0.2 of 150 MPa | |

150.0 °C | 140 MPa Show Material materials with Yield strength Rp0.2 of 140 MPa | |

200.0 °C | 135 MPa Show Material materials with Yield strength Rp0.2 of 135 MPa | |

250.0 °C | 132 MPa Show Material materials with Yield strength Rp0.2 of 132 MPa | |

300.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2 of 130 MPa | |

350.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2 of 130 MPa | |

400.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2 of 130 MPa | |

425.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2 of 130 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 100.0 °C | 150 MPa Show Material materials with Yield strength Rp0.2, transverse of 150 MPa |

150.0 °C | 140 MPa Show Material materials with Yield strength Rp0.2, transverse of 140 MPa | |

200.0 °C | 135 MPa Show Material materials with Yield strength Rp0.2, transverse of 135 MPa | |

250.0 °C | 132 MPa Show Material materials with Yield strength Rp0.2, transverse of 132 MPa | |

300.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2, transverse of 130 MPa | |

350.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2, transverse of 130 MPa | |

400.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2, transverse of 130 MPa | |

425.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2, transverse of 130 MPa | |

Unlock all property charts | ||

Yield strength Rp1.0 | 20.0 °C | 205 - 210 MPa Show Material materials with Yield strength Rp1.0 of 205 - 210 MPa |

100.0 °C | 220 MPa Show Material materials with Yield strength Rp1.0 of 220 MPa | |

200.0 °C | 210 MPa Show Material materials with Yield strength Rp1.0 of 210 MPa | |

300.0 °C | 190 MPa Show Material materials with Yield strength Rp1.0 of 190 MPa | |

400.0 °C | 180 MPa Show Material materials with Yield strength Rp1.0 of 180 MPa | |

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -130.0 °C | 1.15E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.15E-5 1/K | |

-75.0 °C | 1.21E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.21E-5 1/K | ||

93.0 °C | 1.39E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.39E-5 1/K | ||

100.0 °C | 1.38E-5 - 1.39E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.38E-5 - 1.39E-5 1/K | ||

200.0 °C | 1.45E-5 - 1.55E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.45E-5 - 1.55E-5 1/K | ||

300.0 °C | 1.49E-5 - 1.58E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 - 1.58E-5 1/K | ||

400.0 °C | 1.52E-5 - 1.6E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.52E-5 - 1.6E-5 1/K | ||

500.0 °C | 1.56E-5 - 1.63E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.56E-5 - 1.63E-5 1/K | ||

600.0 °C | 1.6E-5 - 1.66E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.6E-5 - 1.66E-5 1/K | ||

700.0 °C | 1.64E-5 - 1.7E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.64E-5 - 1.7E-5 1/K | ||

800.0 °C | 1.68E-5 - 1.74E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.68E-5 - 1.74E-5 1/K | ||

900.0 °C | 1.73E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.73E-5 - 1.77E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | -10 - 450 °C Show Material materials with Max service temperature, long of -10 - 450 °C | ||

Melting point | 1170 - 1365 °C Show Material materials with Melting point of 1170 - 1365 °C | Typical for Nickel Copper Alloy | |

Specific heat capacity | 20.0 °C | 427 - 452 J/(kg·K) Show Material materials with Specific heat capacity of 427 - 452 J/(kg·K) | |

100.0 °C | 445 - 461 J/(kg·K) Show Material materials with Specific heat capacity of 445 - 461 J/(kg·K) | ||

200.0 °C | 465 - 473 J/(kg·K) Show Material materials with Specific heat capacity of 465 - 473 J/(kg·K) | ||

300.0 °C | 478 - 484 J/(kg·K) Show Material materials with Specific heat capacity of 478 - 484 J/(kg·K) | ||

400.0 °C | 490 - 495 J/(kg·K) Show Material materials with Specific heat capacity of 490 - 495 J/(kg·K) | ||

500.0 °C | 523 J/(kg·K) Show Material materials with Specific heat capacity of 523 J/(kg·K) | ||

600.0 °C | 544 J/(kg·K) Show Material materials with Specific heat capacity of 544 J/(kg·K) | ||

700.0 °C | 555 J/(kg·K) Show Material materials with Specific heat capacity of 555 J/(kg·K) | ||

800.0 °C | 566 J/(kg·K) Show Material materials with Specific heat capacity of 566 J/(kg·K) | ||

900.0 °C | 577 J/(kg·K) Show Material materials with Specific heat capacity of 577 J/(kg·K) | ||

1000.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | ||

1150.0 °C | 603 J/(kg·K) Show Material materials with Specific heat capacity of 603 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | -130.0 °C | 22 W/(m·K) Show Material materials with Thermal conductivity of 22 W/(m·K) | |

-75.0 °C | 24 W/(m·K) Show Material materials with Thermal conductivity of 24 W/(m·K) | ||

20.0 °C | 21.8 - 26 W/(m·K) Show Material materials with Thermal conductivity of 21.8 - 26 W/(m·K) | ||

100.0 °C | 25.4 - 29.5 W/(m·K) Show Material materials with Thermal conductivity of 25.4 - 29.5 W/(m·K) | ||

200.0 °C | 28.7 - 33 W/(m·K) Show Material materials with Thermal conductivity of 28.7 - 33 W/(m·K) | ||

300.0 °C | 31.9 - 36.5 W/(m·K) Show Material materials with Thermal conductivity of 31.9 - 36.5 W/(m·K) | ||

400.0 °C | 34.7 - 440 W/(m·K) Show Material materials with Thermal conductivity of 34.7 - 440 W/(m·K) | ||

500.0 °C | 38.4 - 44 W/(m·K) Show Material materials with Thermal conductivity of 38.4 - 44 W/(m·K) | ||

600.0 °C | 41.2 - 48.5 W/(m·K) Show Material materials with Thermal conductivity of 41.2 - 48.5 W/(m·K) | ||

700.0 °C | 43.1 - 52 W/(m·K) Show Material materials with Thermal conductivity of 43.1 - 52 W/(m·K) | ||

800.0 °C | 45.1 - 56 W/(m·K) Show Material materials with Thermal conductivity of 45.1 - 56 W/(m·K) | ||

900.0 °C | 47.5 - 58 W/(m·K) Show Material materials with Thermal conductivity of 47.5 - 58 W/(m·K) | ||

1000.0 °C | 50 W/(m·K) Show Material materials with Thermal conductivity of 50 W/(m·K) | ||

1150.0 °C | 52.9 W/(m·K) Show Material materials with Thermal conductivity of 52.9 W/(m·K) | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 5.13E-7 - 5.47E-7 Ω·m Show Material materials with Electrical resistivity of 5.13E-7 - 5.47E-7 Ω·m |

100.0 °C | 5.4E-7 Ω·m Show Material materials with Electrical resistivity of 5.4E-7 Ω·m | |

200.0 °C | 5.55E-7 Ω·m Show Material materials with Electrical resistivity of 5.55E-7 Ω·m | |

300.0 °C | 5.75E-7 Ω·m Show Material materials with Electrical resistivity of 5.75E-7 Ω·m | |

400.0 °C | 5.85E-7 Ω·m Show Material materials with Electrical resistivity of 5.85E-7 Ω·m | |

500.0 °C | 6E-7 Ω·m Show Material materials with Electrical resistivity of 6E-7 Ω·m | |

600.0 °C | 6.18E-7 Ω·m Show Material materials with Electrical resistivity of 6.18E-7 Ω·m | |

700.0 °C | 6.35E-7 Ω·m Show Material materials with Electrical resistivity of 6.35E-7 Ω·m | |

800.0 °C | 6.55E-7 Ω·m Show Material materials with Electrical resistivity of 6.55E-7 Ω·m | |

900.0 °C | 6.75E-7 Ω·m Show Material materials with Electrical resistivity of 6.75E-7 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.5 % Show Material materials with Aluminium of 0.5 % |

Carbon | 0.15 - 0.3 % Show Material materials with Carbon of 0.15 - 0.3 % |

Cobalt | 2 % Show Material materials with Cobalt of 2 % |

Copper | 28 - 34 % Show Material materials with Copper of 28 - 34 % |

Iron | 1 - 2.5 % Show Material materials with Iron of 1 - 2.5 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Nickel | 63 % Show Material materials with Nickel of 63 % |

Silicon | 0.5 % Show Material materials with Silicon of 0.5 % |

Sulfur | 0.02 - 0.024 % Show Material materials with Sulfur of 0.02 - 0.024 % |

Titanium | 0.3 % Show Material materials with Titanium of 0.3 % |